commutator in Eq. 7.16, which includes the instantaneous selfenergy contributions, reads

id

dt G^{<,cc}(t) = Σ^{δ,cc} G^{<,cc}−G^{<,cc}Σ^{δ,cc}

+ Σ^{δ,cv}G^{<,vc}−G^{<,cv} Σ^{δ,vc}

(7.17a) id

dt G^{<,vv}(t) = Σ^{δ,vc} G^{<,cv}−G^{<,vc}Σ^{δ,cv}

+ Σ^{δ,vv}G^{<,vv} −G^{<,vv}Σ^{δ,vv}

(7.17b) id

dt G^{<,cv}(t) = Σ^{δ,cc} G^{<,cv} −G^{<,cc}Σ^{δ,cv}

+ Σ^{δ,cv}G^{<,vv}−G^{<,cv} Σ^{δ,vv}

(7.17c) id

dt G^{<,vc}(t) = id

dt [G^{<,cv}(t)]^{†} (7.17d)

with the band indices given explicitly. The lesser GFsG^{<,}^{cv}represent inter-band transition
amplitudes that are diagonal and off-diagonal in the state index, i.e. direct and indirect
inter-band transitions. On the other hand the intra-band quantities are given byG^{<,cc}_{αβ} and
G^{<,vv}_{αβ} , describing the population forα = β and intra-band transition amplitudes forα =
β. In Eq. (7.17), state and subband indices are still to be understood in matrix notation
according to

A^{cc} =

⎡

⎢⎢

⎣

ν^{c}ν^{c} ν^{c}**k**^{c}
**k**^{c}ν^{c} **k**^{c}**k**^{c}

⎤

⎥⎥

⎦ , A^{cv} =

⎡

⎢⎢

⎣

ν^{c}ν^{v} ν^{c}**k**_{1}^{v} ν^{c}**k**^{v}_{2}
ν^{c}**k**_{1}^{c} **k**^{c}_{1}**k**^{v}_{1} **k**^{c}_{2}**k**^{v}_{2}

⎤

⎥⎥

⎦ ,

A^{vc} = [A^{cv}]^{†} , A^{vv} =

⎡

⎢⎢

⎢⎢

⎢⎢

⎢⎢

⎣

ν^{v}ν^{v} ν^{v}**k**^{v}_{1} ν^{v}**k**^{v}_{2}
ν^{v}**k**^{v}_{1} **k**_{1}^{v}**k**_{1}^{v} **k**^{v}_{2}**k**_{1}^{v}

ν^{v}**k**^{v}_{2} **k**_{1}^{v}**k**_{2}^{v} **k**^{v}_{2}**k**_{2}^{v}

⎤

⎥⎥

⎥⎥

⎥⎥

⎥⎥

⎦

. (7.18)

Here, ν^{λ} indicates a QD state and **k**_{n}^{λ} a WL state of the n-th subband, with λ
represent-ing the correspondrepresent-ing band. In this example one conduction band and two subbands of
the valence band are considered. Please note, that the QD states occur only once, even
though the valence band contains two subbands. Furthermore the matrix notation implies
a ”sum” over all states in the system. Depending on the sub-blocks of the matrices that are
multiplied with each other in Eq. 7.17, this ”sum” is to be understood either as an
integra-tion _{(2π)}^{1} _{2}

d^{2}kover a continuum of WL states or a summation

**R,ν** over QD states and
positions.

**Instantaneous selfenergy contributions**

As instantaneous selfenergy contributions we consider in the following the free-particle energy dispersion, the optical pulse excitation, and Coulomb renormalizations in SX-CH approximation. A detailed discussion of the different selfenergy contributions is presented in Chap. 4. Consequently, only a short summary is given, where nitride-speciﬁc properties are discussed.

The energy dispersionε^{λ}_{α} we consider for the calculation is depicted in Fig. 7.10 and
in-cluded by means of the selfenergy

Σ^{free}_{αβ}^{,λλ}^{} =ε^{λ}_{α}δ_{αβ} δ_{λλ} . (7.19)
Off-diagonal dipole transitions are driven by the optical pulse, which is included via the
selfenergy (4.50). Only those transition amplitudesG^{<,cv}_{αβ} are driven whose corresponding
dipole matrix elementsd^{cv}_{αβ} are nonzero. For InGaAs QDs the selfenergyΣ^{δ} = Σ^{free}+Σ^{pulse}
is diagonal in the state index. In this case no off-diagonal elements of G^{<}_{αβ} are driven in
the SBE (7.16), even in the presence of two valence bands. For InN QDs where also the
off-diagonal dipole coupling for the QD states is taken into account, the corresponding
interband transition amplitudes G^{<,cv} are driven by the pulse directly. Other inter- and
intra-band transition amplitudes can be driven indirectly, for example via the Coulomb
interaction.

The Coulomb interaction is considered by means of the SX-CH selfenergy (4.19) and
(4.20), as well as the Hartree contributions (4.12). To facilitate the discussion of
off-diagonal contributions, let us ﬁrst focus on the diagrammatic representation of the Hartree
terms is depicted in Fig. 4.3b. As we are restricting ourselves to interaction vertices
diag-onal in the band index, only population functions^{3} appear in the Hartree terms. Were we
to include all possible band-index combinations in the overlaps, also Hartree contributions
containing interband transition amplitudes would appear. The corresponding diagrammatic
representation for the SX-CH selfenergy is depicted in Fig. 4.3a. Due to the off-diagonal
nature of the main QD transitions, cf. the dipole selection rules, the selfenergy for the WL
states reads

Σ^{λλ}_{kk}^{}(t) = i

νμ

V_{kνkμ}^{λλ}^{} G^{<,λλ}_{μν} ^{}(t) + i

**k**^{}

V_{kk}^{λλ}^{}**kk**^{}G^{<,λλ}_{k}_{}_{k}_{}^{}(t), (7.20)
where all GFs G^{<,cv}_{δγ} involving two QD states are non-vanishing and hence all interaction
matrix elementsV_{kγkδ}^{λλ}^{} are required. As the WL-WL overlaps (7.14) contain the momentum
conservation, we can restrict our analysis to diagonal WL GFsG^{≷}** _{kk}**. Note, that inV

_{kk}^{λλ}

^{}

**kk**

^{}

we have to deal with the problem of lifting the Coulomb singularity. The procedure we

3In principle also intra-band transitions amplitudes.

use is discussed in Refs. [64] and an extension to the TB approach is outlined in App. B.4.

Likewise we ﬁnd for the QD states
Σ^{λλ}_{νμ}^{}(t) = i

**k**

V_{νkμk}^{λλ}^{} G^{<,λλ}_{kk}^{}(t) + i

χξ

V_{νχμξ}^{λλ}^{} G^{<,λλ}_{ξχ} ^{}(t), (7.21)
where all QD-QD couplingsV_{νχμξ}^{λλ}^{} are included.

The complicated interplay of all transition amplitudes via the Coulomb matrix elements
poses the question, whether transition amplitudes that are not directly driven by the optical
ﬁeld via the dipole interaction can be driven indirectly via the Coulomb interaction. To
in-vestigate this, let us consider for example the dynamics of a interband transition amplitude
connecting QD and WL statesG^{<,cv}_{νk} . The corresponding equation of motion for this GF
reads

id

dtG^{cv}_{νk}(t) = i

+ Σ^{cc}_{νk}G^{cv}_{kk}+ Σ^{cv}_{νk}G^{vv}_{kk}
+ Σ^{cc}_{νν}G^{cv}_{νk}+ Σ^{cv}_{νν}G^{vv}_{νk}

−G^{cc}_{νk}Σ^{cv}_{kk}−G^{cv}_{νk}Σ^{vv}_{kk}

−G^{cc}_{νν}Σ^{cv}_{νk}−G^{cv}_{νν}Σ^{vv}_{νk}

, (7.22)

where the indices k and ν are to be understood symbolically for the respective state
be-longing either to the WL or to a QD. Furthermore the≷ components are suppressed for
simplicity. All contributions that drive this polarization are proportional to a polarization
times a population. Therefore, in the linear regime, i.e. χ^{(1)}, these terms are not driven
in the limit of vanishing background carrier density. Considering ﬁnite background carrier
densities, e.g. for gain calculations, these terms in principle have to be taken into account.

However, all transition amplitudes not directly driven by the optical pulse, i.e.d_{αβ} = 0, do
not directly contribute to the macroscopic polarization (6.5). Their inﬂuence is restricted
to the back-action on directly driven polarizations. To simplify the numerical evaluation,
we therefore neglect these transition amplitudes in the following. Similar to the discussion
for the Hartree terms, the inclusion of band off-diagonal vertices implies additional terms.

**7.4.2 Linear absorption**

The linear absorption spectrum is calculated from the macroscopic polarization viaχ(ω) =

P(ω)E(ω) ∝ α(ω)as discussed in Chap. 6.1. As the SX-CH and the Hartree selfenergies we consider for the calculation do not provide microscopic dephasing, in a ﬁrst step we use a phenomenological value of γ =10 meV. Calculations that additionally include micro-scopic dephasing due to carrier-LO-phonon collisions are presented below. In comparison to typical InGaAs QDs discussed in previous chapters, the InN QD under consideration exhibits deeply conﬁned shells, especially for electrons, cf. Fig. 7.10. The conﬁnement

energy for the lowest QD states with respect to the band edge is -575.4 meV and -345.3 meV for electrons, and -49.6 meV and -39.8 meV for holes. In conjunction with the ”skew”

dipole selection rules discussed in Chap. 7.2.5, this corresponds to free-carrier transition energies of -615.2 meV and -394.9 meV, relative to the WL bandgap of 1731 meV. As initial carrier distribution, we assume a quasi-equilibrium situation for the CB as well as a common one for the two VBs.

1000 1200 1400 1600

energy in meV 0

2 4 6 8 10

absorption in arb. units

7.0e09 cm^{-2}
1.2e10
1.7e10
2.0e10
5.0e10
2.0e11

**Fig. 7.15: Linear optical absorption spectra for InN QDs at 300 K and for various carrier**
densities, considering a phenomenological dephasing of 10 meV.

The corresponding absorption spectra for a temperature of 300 K and various carrier
densi-ties are shown in Fig. 7.15. With increasing carrier density, the transition energies exhibit
a blue shift accompanied by bleaching of the absorption and transition to gain. For carrier
densities exceeding 5×10^{10}cm^{−2} the blue shift is reduced. This complicated behavior
is due to the interplay of Hartree, screened-exchange (SX) and Coulomb hole (CH)
con-tributions. The corresponding numbers for three exemplary carrier densities are given in
Tab. 7.2. As we can infer, the CH energy shifts are practically the same for CB and VB
carriers and therefore only slightly inﬂuence the interband transition energies. In contrast,
Hartree as well as SX terms give rise to a relative shift of CB and VB energies. Since
for each band the Hartree term contains contributions from all bands (cf. Eq. (4.12) and
Fig. 4.3b), the inﬂuence of the QD population on the Hartree shift is similar for CB and
VB. The large difference between CB and VB shifts arises from the screened interaction
matrix elements. The blue shift for small to intermediate carrier densities stems from the
steep increase of the Hartree contributions. For larger carrier densities, the Hartree terms
saturate due to ﬁlling of the QD states. Simultaneously the screening of the Coulomb

2×10^{10}cm^{−2} 5×10^{10}cm^{−2} 2×10^{11}cm^{−2}

**CB** SX 1 -73.7 -88.9 -64.5

SX 2 -17.5 -58.3 -46.3

CH 1 -14.1 -20.1 -36.5

CH 2 -13.3 -18.6 -31.9

H 1 149.0 285.5 189.4

H 2 124.8 245.7 156.2

**VB** SX 1 2.9 6.4 15.4

SX 2 2.4 5.4 14.4

CH 1 -13.9 -19.7 -35.6

CH 2 -14.0 -19.9 -36.3

H 1 -13.3 -29.1 -70.1

H 2 -14.4 -31.7 -79.1

**Tab. 7.2: Energy shift contributions from screened-exchange (SX), Coulomb hole (CH),**
and Hartree (H) selfenergies in meV.

interaction increases due to ﬁlling of WL states which leads to a strong reduction of the Hartree contributions. In contrast, saturation effects are smaller for the SX terms because of increasing contributions from WL carriers. This leads in total to a reduced blue shift for high carrier densities.

To employ a microscopic dephasing mechanism we consider the interaction with LO phonons, where, similar to the extended discussion in Chap. 5.2.2, we use the RPA selfen-ergy. Speciﬁcally, we consider the one-time collision terms (3.72) in the Markovian limit which is obtained by application of the reverse GKBA, cf. Chap. 3.5. This procedure

yields d

dtG^{<,cv}_{αβ} (t)

coll = ^{2}

γδξ

**q**

t

−∞

dt_{3}

+ G^{cc,>}_{δξ} (t)G^{c,}_{ξ}^{R}(t, t_{3})D_{αξγδ,q}^{cccc,<}(t_{3}, t)G^{c,}_{γ}^{A}(t_{3}, t)G^{cv,<}_{γβ} (t)

− G^{cc,<}_{δξ} (t)G^{c,}_{ξ}^{R}(t, t_{3})D^{cccc,>}_{αξγδ,q}(t_{3}, t)G^{c,A}_{γ} (t_{3}, t)G^{cv,>}_{γβ} (t)
+ G^{cc,<}_{αγ} (t)G^{c,R}_{γ} (t, t_{3})G^{c,A}_{δ} (t_{3}, t)G^{cv,>}_{δξ} (t)D_{γξβδ,q}^{cvvc,<}(t, t_{3})

− G^{cc,>}_{αγ} (t)G^{c,}_{γ}^{R}(t, t_{3})G^{c,}_{δ}^{A}(t_{3}, t)G^{cv,<}_{δξ} (t)D_{γξβδ,q}^{cvvc,>}(t, t_{3})
+ G^{cv,>}_{δξ} (t)G^{v,}_{ξ}^{R}(t, t_{3})D^{cvvc,<}_{αξγδ,q}(t_{3}, t)G^{v,}_{γ}^{A}(t_{3}, t)G^{vv,<}_{γβ} (t)

− G^{cv,<}_{δξ} (t)G^{v,}_{ξ}^{R}(t, t_{3})D^{cvvc,>}_{αξγδ,q}(t_{3}, t)G^{v,A}_{γ} (t_{3}, t)G^{vv,>}_{γβ} (t)
+ G^{cv,<}_{αγ} (t)G^{v,R}_{γ} (t, t_{3})G^{v,}_{δ}^{A}(t_{3}, t)G^{vv,>}_{δξ} (t)D_{γξβδ,q}^{vvvv,<}(t, t_{3})

− G^{cv,>}_{αγ} (t)G^{v,}_{γ}^{R}(t, t_{3})G^{v,}_{δ}^{A}(t_{3}, t)G^{vv,<}_{δξ} (t)D^{vvvv,>}_{γξβδ,q}(t, t_{3})
.
(7.23)
withD_{αβγδ}(t_{1}, t_{2})containing the interaction matrix elements as well as the phonon
propa-gator, cf. Eq. 4.32. Also in this case a separation into diagonal and off-diagonal dephasing
is possible, even though the situation is more complicated due to the coupling of different
off-diagonal GFs. Nevertheless, a compensation between the two contributions also holds
in this case.

The corresponding optical absorption spectra including dephasing due to LO-phonon col-lisions are presented in Fig. 7.16. Energy shifts due to polaron effects are small in compar-ison to SX-CH and Hartree interaction which are identical as in the results shown above.

The main inﬂuence of carrier-phonon scattering is dephasing of the optical polarization that corresponds to broadening of the resonances. An asymmetric line shape as well as a typical line width of 22 meV for the energetically lower and 18 meV for the energetically higher transition are found. The difference arises due to the fact that for the energetically lower transition the off-diagonal compensation is reduced due to the large energetic sepa-ration from the WL. It should be noted, that at the low energy side of the QD resonances a slightly negative absorption is observed. This artifact we attribute to the GKBA, since as shown in Chap. 5.3.3 the validity of the GKBA for intermediate to strong polar coupling materials is questioned.

1000 1200 1400 1600 energy in meV

0 2 4 6 8 10

absorption in arb. units

7.0e09 cm^{-2}
1.2e10
1.7e10
2.0e10
5.0e10
2.0e11

**Fig. 7.16: Linear optical absorption spectra for InN QDs at 300 K and for various carrier**
densities. The dephasing is provided by carrier-LO-phonon collisions and included on a
microscopic basis.

**7.4.3 Dephasing due to Coulomb scattering**

Absorption spectra for InGaAs QDs are presented in Chap. 6.1. To determine excitation-induced dephasing due to Coulomb interaction the second Born approximation (SBA) was employed, cf. Chap. 4.1. In contrast, for the nitride material system we use the SX-CH approximation. Therefore several comments on important differences between the two approaches are in order.

t_{1} t_{1} t_{1}

(a) SX-CH

t_{1} t_{2} t_{1}

(b) direct SBA

t_{1} t_{2} t_{1}

(c) exchange SBA

**Fig. 7.17: Schematic representation of SX-CH diagrams SBA diagrams.**

Schematically, the contributing diagrams in the Kadanoff-Baym equations (3.64) are
de-picted in Fig. 7.17. In contrast to the usual notation, the wiggly interaction line denotes the
retarded/advanced plasmon GFW^{R}^{/}^{A} and the carrier propagators G^{≷}are represented by

straight lines. Therefore, these diagrams should not be confused with Feynman diagrams
as no systematic perturbation expansion is implied. For the following discussion note, that
W^{R}^{/}^{A} is a real quantity under the assumption that the screening is instantaneous and does
not contain retardation effect, cf. the discussion in Chap. A.2. Considering the
homoge-neous part of the equation of motion for the polarization, i^{dψ}_{dt} = Δψ, the dephasing is
identiﬁed as the imaginary part ofΔ. In the SX-CH selfenergy diagram (cf. Fig. 7.17a) no
retardation effects are included due to the instantaneous interaction and hence all internal
times are ﬁxed to the external ones. This implies the structureΔ∝W^{R/A}f, which is a real
quantity and hence provides no dephasing. In contrast, in the SBA diagrams an internal
time t_{2} is involved (cf. Fig. 7.17b,c). Hence, retardation effects, that are included in the
two-time propagatorsG^{≷}(t_{1}, t_{2}), contribute. This can be easily seen when representing the
two-time propagator by means of the GKBA, which maps the two-time propagators onto
the time-diagonal with the help of retarded/advanced GFs, cf. Chap. 3.5. For the equation
of motion this implies the structureΔ =W W^{∗}f f f G^{R}G^{R}G^{R}G^{R}, which is complex in
gen-eral, and hence provides dephasing. However, the inclusion of dephasing due to Coulomb
scattering in our calculations for nitride semiconductors remains a challenging task as in
addition to the calculations shown in Chap. 6.1 one has to account for off-diagonal GFs.

Moreover, in the calculations for the InGaAs material using the harmonic-oscillator model (cf. Chap. A.1) the matrix elements to a large extend can be calculated analytically, which is not possible in the nitride case and thus by far enhancing the computational effort.

This thesis provides a deeper insight into to carrier-LO-phonon scattering mechanism in semiconductor QDs. On the one hand the interaction gives rise to renormalizations of the single-particle states, and on the other hand it leads to carrier scattering and dephasing processes. The interplay of these two effects was studied using the framework of non-equilibrium Green’s functions.

Most important for the understanding of scattering and dephasing mechanism are the renor-malizations of the single-particle states. In case of the carrier-LO-phonon interaction, they are described by the formation of polarons. An intuitive approach for the discussion of polarons is the spectral function, which is connected to the density of states. For con-tinuous systems like QWs, the spectral function is dominated by a single resonance. In this case results from perturbation theory are in good agreement with our non-perturbative approach, leading simply to a shift of the free-particle energies and introducing a ﬁnite carrier lifetime. In contrast, for QD systems perturbation theory clearly fails. The carrier conﬁnement gives rise to an enhanced effective coupling, resulting in pronounced phonon satellites and their hybridization. Strong coupling effects are observed, even for weak polar coupling materials. Additionally, the interaction of QD states with the energetically close continuum of WL states leads to a further broadening of the polaron resonances at room temperature. In contrast, at low temperatures only a few phonons are present. As a con-sequence, phonon absorption processes are strongly suppressed and emission processes dominate. This leads to a much weaker interaction between QD and WL states, resulting in much narrower resonances of the spectral function.

These polaron properties determine to a large extent the efﬁciency of carrier-scattering processes, as the scattering kernel is given by the overlap of the spectral functions of the involved states. Thus, within the quasi-particle picture of carrier-scattering a deeper in-sight into the phonon-bottleneck controversy was achieved. Because of the controversial experimental ﬁndings regarding the phonon-bottleneck discussion, further investigations have been performed. For elevated temperatures we ﬁnd that polaron effects give rise to fast scattering channels, whereas in the low-temperature regime an initial fast relaxation is followed by a freezing of the carrier distribution at later times, not reaching a thermal dis-tribution. Thus, our analysis shows that the phonon bottleneck discussion in QDs should include the energy spectrum of the QD, the temperature regime, and the timescales in-volved. The question about the presence of a phonon bottleneck can not be answered by the energy mismatch argument alone. As applications of the developed quantum-kinetic

model we have presented an investigation of the inﬂuence of carrier-phonon scattering on the optical response by means of absorption spectra and the temporally resolved photolu-minescence. The analysis of the optical response, including dephasing processes due to both, carrier-carrier and carrier-phonon interaction, showed that it is essential to consider quasi-particle renormalizations in a self-consistent way. Furthermore it was found that both contributions to the dephasing are important, even in the high carrier-density regime.

For the nitride material system it turned out that, besides many-body effects, a micro-scopic treatment of the electronic properties is of central importance, as intrinsic and strain-induced electric ﬁelds as well as the QD geometry and the underlying wurtzite crystal structure strongly inﬂuence the electronic properties. To study the interplay of the par-ticular single-particle wave functions and many-body effects, a procedure to incorporate results from an atomistic tight-binding approach into our quantum-kinetic theory was de-veloped. As a ﬁrst application the properties of nitride polarons have been investigated. In a second step absorption spectra are presented where we considered Coulomb renormaliza-tions as well as the dephasing due to carrier-phonon interaction including polaron effects.

These results show large excitation-induced shifts of the QD resonances, which deﬁnitely have to be considered for practical applications like LEDs and laser diodes.

**Future directions**

The results presented in this thesis may serve as a starting point for further investigations in the ﬁeld of quantum kinetics and semiconductor quantum dot systems. Whereas the one-time kinetics provides an intuitive way to incorporate memory effects and quasi-particle renormalizations, intrinsic shortcomings of the involved GKBA, in particular for interme-diate to strong polar coupling materials, should be investigated further. Such investigations might for example include new quasi-particle concepts presented by Velický et al. [89], a more detailed analysis of the reconstruction scheme for two-time propagators, and a further analysis of the two-time equations including the kinetics of individual polaron satellites.

For the carrier scattering a calculation of the temporal evolution of the population distri-bution including both, carrier-carrier and carrier-phonon interaction, would be interesting, especially since the relaxation times we computed indicate that in QD systems even at low carrier densities Coulomb scattering is not negligible. With the new generation of CPU clusters such calculations in a one-time version should be feasible. Another aspect for the optical response of semiconductor QDs is the exciton phonon interaction, represented by selfenergy diagrams that contain both carrier-carrier and carrier-phonon interaction lines.

Such contributions, giving rise to phonon replica of the exciton resonances in the optical spectra, are clearly observed in experimental data. Furthermore, the procedure presented to incorporate wave functions obtained from atomistic tight-binding calculations opens a whole ﬁeld of future investigations. For the nitride material system, especially the inﬂu-ence of speciﬁc material compositions, e.g. ternary alloys, concentration gradients due to

tions, QD geometry and strain, obtained for example with a transmission-electron micro-scope. Using these data as input for a tight-binding calculation, immediately enables us to determine the optical response including many-body effects.

**Appendix**

**and additional material**

**A.1 Envelope wave function model**

Based on the symmetry properties of the QD-WL system, one assumes for the wave func-tions in Bloch representation a factorization of the envelope function into an 2D in-plane partϕ(ρ)and an 1D partξ(z)in growth direction,

ψ(r) =ϕ(ρ)ξ(z)u** _{k≈0}**(r), (A.1)

with the lattice periodic Bloch functionu** _{k≈0}**(r). The envelope part in growth direction is
described by a 1D quantum well (QW) wave function, where only the lowest subband is
taken into account. The simplest approach would be to consider QW barriers of inﬁnite
height, where the eigenfunctions are known analytically, ξ(z) = sin-

_{π}

Lz.

. Considering barriers of ﬁnite height or a more complicated potential to incorporate e.g. the Quantum conﬁned Stark effect (see Chap. 7.1), the envelope part is evaluated numerically by dis-cretization of the corresponding 1D Schrödinger equation in real space, see e.g. [202, 203].

In the absence of QDs, the delocalized states are described by 2D plane waves (PW)

ϕ^{0}** _{k}**() = √1

A e^{ik}, (A.2)

with**k**being the 2D in-plane momentum. Considering ﬂat, lens-shaped quantum dots, the
in-plane conﬁnement potential was shown to be harmonic in good approximation [140,
204]. The corresponding 2D harmonic oscillator wave functions are well known [29] and
classiﬁed by their angular momentum properties. Correspondingly they are referred to as

s-, p- and d-shell.

ϕ^{s}_{m=0}(−**R) =** β

√π e^{−}^{β}

2|−R|2

2 , (A.3a)

ϕ^{p}_{m=±1}(−**R) =** β

√π e^{−}^{β}

2|−R|2

2 ·β|−**R|**e^{±iφ}, (A.3b)

ϕ^{d}_{m=±2}(−**R) =** β

√π e^{−}^{β}

2|−R|2

2 · (β |−**R|)**^{2} e^{±i2φ}, (A.3c)
ϕ^{d}_{m=0}(−**R) =** β

√π e^{−}^{β}^{2}^{|−R|}^{2} ^{2} · (β(−**R|)**^{2}−1

(A.3d)
In this notation **R** is the position of the QD on the WL plane and β = ^{√}^{mΔE}_{} is the
inverse oscillator length, determining the equidistant energy separationΔE between the
QD shells.

**Interaction matrix elements**

According to the separation ansatz (A.1), thez-dependence in the bare Coulomb interac-tion matrix elements (4.1) might be cast into a formfactor,

V_{1234} = e^{2}
4πε_{0}

d^{2}q 1

**q** F_{1234}(q) φ_{1}|e^{iqρ}|φ_{4} φ_{2}|e^{−iqρ}|φ_{3} (A.4)
with

F_{1234}(q) =

dz

dz^{} ξ(z)ξ(z^{})e^{iq}^{z} ^{(z−z}^{}^{)}ξ(z^{})ξ(z). (A.5)
The overlap integrals for the QD-WL system under consideration are discussed below.

Note, that the Carrier-LO-phonon interaction matrix elements and the bare Coulomb inter-action matrix elements are connected according to (4.37).

**Orthogonalized plane waves**

As for the in-plane part the harmonic oscillator states and the plane waves are orthogo-nal among themselves but not among each other, the orthogoorthogo-nalized-plane-waves (OPW) scheme is applied,

|k= 1
N_{k}

|k_{0} −

ν,R

|ν,**R **ν,**R|k**_{0}

, (A.6)

N** _{k}** =

1−N

ν

| k_{0}|ν |^{2} . (A.7)

Here, explicitly the random distribution of QDs on the WL plane was used. Since the QD
position only gives rise to a phase factor ν,**R|k**0 = ν|k0 e^{ikR}, on average
momen-tum conservation is restored, k|k^{} ∝ δ(k −**k**^{}). Keeping in mind that k_{0}|ν ∝ ^{√}^{1}_{A},
effectively only the QD densityN_{QD} = ^{N}_{A} enters the theory.

In principle the OPW scheme also leads to a modiﬁcation of the energies of the WL states.

However, this change can be neglected if the QD density and the QD size are sufﬁciently small or, in other words, if the fraction of the WL plane that is covered with QDs is sufﬁ-ciently small. Consider the expectation value of the total energy for the total Hamiltonian containing QD and WL states,

k|H|k=k0|H|k0 −N

ν

k0|H|ν ν|k0 −N

ν

k0|ν ν|H|k0

+N

ν,μ

k0|ν ν|H|μ μ|k0

=k_{0}|H|k_{0} −N

ν

E_{ν}| ν|k_{0} |^{2} . (A.8)

Taking into account that the overlaps| ν|k_{0} |^{2}contain factors of _{A}^{1}, we ﬁnd that in the last
line the second term is proportional to the QD densityN_{QD}. This shows that for sufﬁciently
low QD densities (in the sense explained above), we can disregard the OPW corrections to
the WL energies. As the WL energies in the presence of QDs are not known, we work in
good approximation work with the PW energiesk0|H|k0 ≈E_{k}^{0}. However, as the matrix
elements calculated from non-orthogonal states lead to clear deviations in the results, it is
essential to include the OPW corrections to the wave-functions.

**Overlap integrals**

For the calculation of Coulomb and Fröhlich interaction matrix elements, see Chap. 4,
overlap integrals of the formα|e^{iqr}|βhave to be evaluated. Using the OPW scheme and
assuming identical QDs, we ﬁnd for the QD-WL overlaps

ν|e^{iqr}|k= 1
N_{k}

ν|e^{iqr}|k_{0} −

ν^{}

ν|e^{iqr}|ν^{} ν^{}|k_{0}

, (A.9)

and for the WL-WL overlaps

k|e^{iqr}|k^{}=δ(q+**k**^{}−**k)**D_{OPW}(k,**q**,**k**^{}), (A.10)